#------------------------------------------------------------------------------
#$Date: 2017-04-03 22:24:16 +0300 (Mon, 03 Apr 2017) $
#$Revision: 194660 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/51/40/4514077.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4514077
loop_
_publ_author_name
'Wang, Bin'
'Yang, Qi'
'Guo, Chao'
'Sun, Yuxiu'
'Xie, Lin-Hua'
'Li, Jian-Rong'
_publ_section_title
;
 Stable Zr(IV)-Based Metal-Organic Frameworks with Predesigned
 Functionalized Ligands for Highly Selective Detection of Fe(III) Ions in
 Water.
;
_journal_issue                   11
_journal_name_full               'ACS applied materials & interfaces'
_journal_page_first              10286
_journal_page_last               10295
_journal_paper_doi               10.1021/acsami.7b00918
_journal_volume                  9
_journal_year                    2017
_chemical_formula_sum            'C44 H24 N2 O16 Zr3'
_chemical_formula_weight         1110.31
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           141
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   20.6568(3)
_cell_length_b                   20.6568(3)
_cell_length_c                   66.6868(14)
_cell_measurement_reflns_used    6738
_cell_measurement_temperature    100.00(10)
_cell_measurement_theta_max      72.4050
_cell_measurement_theta_min      3.9210
_cell_volume                     28455.5(8)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100.00(10)
_diffrn_detector                 'CCD plate'
_diffrn_measured_fraction_theta_full 0.982
_diffrn_measured_fraction_theta_max 0.982
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, AtlasS2'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0665
_diffrn_reflns_av_sigmaI/netI    0.0541
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       82
_diffrn_reflns_limit_l_min       -75
_diffrn_reflns_number            39685
_diffrn_reflns_theta_full        74.54
_diffrn_reflns_theta_max         74.54
_diffrn_reflns_theta_min         3.30
_exptl_absorpt_coefficient_mu    1.970
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.78335
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    0.518
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Octahedral
_exptl_crystal_F_000             4400
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.18
_platon_squeeze_details
;
;
_refine_diff_density_max         1.068
_refine_diff_density_min         -0.648
_refine_diff_density_rms         0.059
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.870
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     154
_refine_ls_number_reflns         7576
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      0.902
_refine_ls_R_factor_all          0.0707
_refine_ls_R_factor_gt           0.0455
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0790P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1234
_refine_ls_wR_factor_ref         0.1320
_reflns_number_gt                4650
_reflns_number_total             7576
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            am7b00918_si_002.cif
_cod_data_source_block           BUT_15
_cod_original_sg_symbol_H-M      I41/amd
_cod_database_code               4514077
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y+1/4, x+3/4, z+1/4'
'-x, -y+1/2, z'
'y+1/4, -x+1/4, z+3/4'
'x, -y, -z'
'-x, y+1/2, -z'
'y+1/4, x+3/4, -z+1/4'
'-y+1/4, -x+1/4, -z+3/4'
'x+1/2, y+1/2, z+1/2'
'-y+3/4, x+5/4, z+3/4'
'-x+1/2, -y+1, z+1/2'
'y+3/4, -x+3/4, z+5/4'
'x+1/2, -y+1/2, -z+1/2'
'-x+1/2, y+1, -z+1/2'
'y+3/4, x+5/4, -z+3/4'
'-y+3/4, -x+3/4, -z+5/4'
'-x, -y, -z'
'y-1/4, -x-3/4, -z-1/4'
'x, y-1/2, -z'
'-y-1/4, x-1/4, -z-3/4'
'-x, y, z'
'x, -y-1/2, z'
'-y-1/4, -x-3/4, z-1/4'
'y-1/4, x-1/4, z-3/4'
'-x+1/2, -y+1/2, -z+1/2'
'y+1/4, -x-1/4, -z+1/4'
'x+1/2, y, -z+1/2'
'-y+1/4, x+1/4, -z-1/4'
'-x+1/2, y+1/2, z+1/2'
'x+1/2, -y, z+1/2'
'-y+1/4, -x-1/4, z+1/4'
'y+1/4, x+1/4, z-1/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Zr1 Zr 0.5000 0.2500 0.088340(5) 0.03061(12) Uani 1 4 d S
Zr2 Zr 0.414793(12) 0.335208(12) 0.1250 0.05083(14) Uani 1 2 d S
O1 O 0.43530(10) 0.31374(11) 0.07134(3) 0.0478(5) Uani 1 1 d .
O2 O 0.37428(15) 0.36188(17) 0.09488(3) 0.1014(12) Uani 1 1 d .
O3 O 0.42652(12) 0.2500 0.10926(3) 0.0347(6) Uani 1 2 d S
O4 O 0.5000 0.34831(13) 0.10471(3) 0.0453(7) Uani 1 2 d S
O5 O 0.4203(2) 0.44043(15) 0.12275(4) 0.1359(17) Uani 1 1 d .
N1 N 0.27406(19) 0.5000 0.0000 0.102(2) Uani 1 2 d S
C1 C 0.39077(17) 0.3501(2) 0.07682(5) 0.0672(11) Uani 1 1 d .
C2 C 0.35213(17) 0.3837(2) 0.06107(5) 0.0743(13) Uani 1 1 d .
C3 C 0.37294(18) 0.3825(2) 0.04161(5) 0.0782(13) Uani 1 1 d .
H3 H 0.4113 0.3596 0.0382 0.094 Uiso 1 1 calc R
C4 C 0.33838(17) 0.4146(2) 0.02686(5) 0.0836(15) Uani 1 1 d .
H4 H 0.3553 0.4170 0.0136 0.100 Uiso 1 1 calc R
C5 C 0.27969(17) 0.4431(3) 0.03119(6) 0.0974(18) Uani 1 1 d .
C6 C 0.2584(2) 0.4418(3) 0.05084(6) 0.112(2) Uani 1 1 d .
H6 H 0.2183 0.4614 0.0542 0.134 Uiso 1 1 calc R
C7 C 0.2949(2) 0.4125(3) 0.06554(6) 0.0971(17) Uani 1 1 d .
H7 H 0.2798 0.4124 0.0790 0.117 Uiso 1 1 calc R
C8 C 0.24069(18) 0.4748(3) 0.01510(6) 0.1016(19) Uani 1 1 d .
C9 C 0.17458(17) 0.4741(3) 0.01600(7) 0.131(3) Uani 1 1 d .
H9 H 0.1528 0.4564 0.0273 0.157 Uiso 1 1 calc R
C10 C 0.1398(3) 0.5000 0.0000 0.135(4) Uani 1 2 d S
C11 C 0.0674(3) 0.5000 0.0000 0.195(6) Uani 1 2 d S
C12 C 0.0353(3) 0.4853(4) 0.01460(11) 0.206(3) Uani 1 1 d U
H12 H 0.0572 0.4733 0.0266 0.247 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0311 0.0180 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zr Zr -0.1862 2.2449 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Zr1 O3 94.84(13) 3_655 .
O3 Zr1 O1 143.02(6) 3_655 22_565
O3 Zr1 O1 84.31(7) . 22_565
O3 Zr1 O1 84.31(7) 3_655 21_655
O3 Zr1 O1 143.02(6) . 21_655
O1 Zr1 O1 117.73(10) 22_565 21_655
O3 Zr1 O1 84.31(7) 3_655 3_655
O3 Zr1 O1 143.02(6) . 3_655
O1 Zr1 O1 75.14(11) 22_565 3_655
O1 Zr1 O1 73.84(12) 21_655 3_655
O3 Zr1 O1 143.02(6) 3_655 .
O3 Zr1 O1 84.31(7) . .
O1 Zr1 O1 73.84(12) 22_565 .
O1 Zr1 O1 75.14(11) 21_655 .
O1 Zr1 O1 117.73(10) 3_655 .
O3 Zr1 O4 71.32(5) 3_655 .
O3 Zr1 O4 71.32(5) . .
O1 Zr1 O4 140.71(6) 22_565 .
O1 Zr1 O4 73.48(7) 21_655 .
O1 Zr1 O4 140.71(6) 3_655 .
O1 Zr1 O4 73.48(7) . .
O3 Zr1 O4 71.32(5) 3_655 3_655
O3 Zr1 O4 71.32(5) . 3_655
O1 Zr1 O4 73.48(7) 22_565 3_655
O1 Zr1 O4 140.71(6) 21_655 3_655
O1 Zr1 O4 73.48(7) 3_655 3_655
O1 Zr1 O4 140.71(6) . 3_655
O4 Zr1 O4 123.48(12) . 3_655
O3 Zr1 Zr2 32.27(2) 3_655 26_565
O3 Zr1 Zr2 84.11(6) . 26_565
O1 Zr1 Zr2 166.65(5) 22_565 26_565
O1 Zr1 Zr2 75.62(5) 21_655 26_565
O1 Zr1 Zr2 110.96(5) 3_655 26_565
O1 Zr1 Zr2 111.52(6) . 26_565
O4 Zr1 Zr2 39.09(4) . 26_565
O4 Zr1 Zr2 96.47(5) 3_655 26_565
O3 Zr1 Zr2 84.11(6) 3_655 20_656
O3 Zr1 Zr2 32.27(2) . 20_656
O1 Zr1 Zr2 75.62(5) 22_565 20_656
O1 Zr1 Zr2 166.65(5) 21_655 20_656
O1 Zr1 Zr2 111.52(6) 3_655 20_656
O1 Zr1 Zr2 110.96(5) . 20_656
O4 Zr1 Zr2 96.47(5) . 20_656
O4 Zr1 Zr2 39.09(4) 3_655 20_656
Zr2 Zr1 Zr2 91.032(11) 26_565 20_656
O3 Zr1 Zr2 84.11(6) 3_655 .
O3 Zr1 Zr2 32.27(2) . .
O1 Zr1 Zr2 110.96(5) 22_565 .
O1 Zr1 Zr2 111.52(6) 21_655 .
O1 Zr1 Zr2 166.65(5) 3_655 .
O1 Zr1 Zr2 75.62(5) . .
O4 Zr1 Zr2 39.09(4) . .
O4 Zr1 Zr2 96.47(5) 3_655 .
Zr2 Zr1 Zr2 60.594(6) 26_565 .
Zr2 Zr1 Zr2 60.594(6) 20_656 .
O3 Zr1 Zr2 32.27(2) 3_655 3_655
O3 Zr1 Zr2 84.11(6) . 3_655
O1 Zr1 Zr2 111.52(6) 22_565 3_655
O1 Zr1 Zr2 110.96(5) 21_655 3_655
O1 Zr1 Zr2 75.62(5) 3_655 3_655
O1 Zr1 Zr2 166.65(5) . 3_655
O4 Zr1 Zr2 96.47(5) . 3_655
O4 Zr1 Zr2 39.09(4) 3_655 3_655
Zr2 Zr1 Zr2 60.594(6) 26_565 3_655
Zr2 Zr1 Zr2 60.594(6) 20_656 3_655
Zr2 Zr1 Zr2 91.032(11) . 3_655
O3 Zr2 O3 93.36(13) . 26_565
O3 Zr2 O5 143.96(8) . .
O3 Zr2 O5 96.16(14) 26_565 .
O3 Zr2 O5 96.16(14) . 16_554
O3 Zr2 O5 143.96(8) 26_565 16_554
O5 Zr2 O5 96.2(2) . 16_554
O3 Zr2 O4 69.56(7) . 20_656
O3 Zr2 O4 72.72(9) 26_565 20_656
O5 Zr2 O4 146.29(8) . 20_656
O5 Zr2 O4 78.28(12) 16_554 20_656
O3 Zr2 O4 72.72(9) . .
O3 Zr2 O4 69.56(7) 26_565 .
O5 Zr2 O4 78.28(12) . .
O5 Zr2 O4 146.29(8) 16_554 .
O4 Zr2 O4 123.82(13) 20_656 .
O3 Zr2 O2 78.34(10) . .
O3 Zr2 O2 143.33(9) 26_565 .
O5 Zr2 O2 73.35(13) . .
O5 Zr2 O2 72.71(10) 16_554 .
O4 Zr2 O2 133.58(12) 20_656 .
O4 Zr2 O2 73.88(9) . .
O3 Zr2 O2 143.33(9) . 16_554
O3 Zr2 O2 78.34(10) 26_565 16_554
O5 Zr2 O2 72.71(10) . 16_554
O5 Zr2 O2 73.35(13) 16_554 16_554
O4 Zr2 O2 73.88(9) 20_656 16_554
O4 Zr2 O2 133.58(12) . 16_554
O2 Zr2 O2 128.14(13) . 16_554
O3 Zr2 Zr1 82.36(6) . 26_565
O3 Zr2 Zr1 32.22(6) 26_565 26_565
O5 Zr2 Zr1 121.63(10) . 26_565
O5 Zr2 Zr1 115.35(7) 16_554 26_565
O4 Zr2 Zr1 40.54(7) 20_656 26_565
O4 Zr2 Zr1 95.05(5) . 26_565
O2 Zr2 Zr1 159.88(7) . 26_565
O2 Zr2 Zr1 71.64(6) 16_554 26_565
O3 Zr2 Zr1 32.22(6) . .
O3 Zr2 Zr1 82.36(6) 26_565 .
O5 Zr2 Zr1 115.35(7) . .
O5 Zr2 Zr1 121.63(10) 16_554 .
O4 Zr2 Zr1 95.05(5) 20_656 .
O4 Zr2 Zr1 40.54(7) . .
O2 Zr2 Zr1 71.64(6) . .
O2 Zr2 Zr1 159.88(7) 16_554 .
Zr1 Zr2 Zr1 88.968(11) 26_565 .
O3 Zr2 Zr2 31.47(5) . 20_656
O3 Zr2 Zr2 83.26(7) 26_565 20_656
O5 Zr2 Zr2 175.05(8) . 20_656
O5 Zr2 Zr2 87.01(12) 16_554 20_656
O4 Zr2 Zr2 38.10(5) 20_656 20_656
O4 Zr2 Zr2 96.95(7) . 20_656
O2 Zr2 Zr2 104.21(9) . 20_656
O2 Zr2 Zr2 111.89(8) 16_554 20_656
Zr1 Zr2 Zr2 59.703(3) 26_565 20_656
Zr1 Zr2 Zr2 59.703(3) . 20_656
O3 Zr2 Zr2 83.26(7) . 26_565
O3 Zr2 Zr2 31.47(5) 26_565 26_565
O5 Zr2 Zr2 87.01(12) . 26_565
O5 Zr2 Zr2 175.05(8) 16_554 26_565
O4 Zr2 Zr2 96.95(7) 20_656 26_565
O4 Zr2 Zr2 38.10(5) . 26_565
O2 Zr2 Zr2 111.89(8) . 26_565
O2 Zr2 Zr2 104.21(9) 16_554 26_565
Zr1 Zr2 Zr2 59.703(3) 26_565 26_565
Zr1 Zr2 Zr2 59.703(3) . 26_565
Zr2 Zr2 Zr2 90.0 20_656 26_565
C1 O1 Zr1 131.51(17) . .
C1 O2 Zr2 134.3(2) . .
Zr1 O3 Zr2 115.51(7) . .
Zr1 O3 Zr2 115.51(7) . 20_656
Zr2 O3 Zr2 117.05(10) . 20_656
Zr2 O4 Zr2 103.80(9) . 26_565
Zr2 O4 Zr1 100.36(8) . .
Zr2 O4 Zr1 100.36(8) 26_565 .
C8 N1 C8 117.4(4) 5_565 .
O1 C1 O2 126.2(3) . .
O1 C1 C2 118.1(3) . .
O2 C1 C2 115.7(3) . .
C7 C2 C3 119.4(3) . .
C7 C2 C1 121.1(3) . .
C3 C2 C1 119.5(3) . .
C2 C3 C4 120.3(4) . .
C2 C3 H3 119.9 . .
C4 C3 H3 119.9 . .
C5 C4 C3 120.6(3) . .
C5 C4 H4 119.7 . .
C3 C4 H4 119.7 . .
C4 C5 C6 118.1(3) . .
C4 C5 C8 120.8(3) . .
C6 C5 C8 121.2(4) . .
C7 C6 C5 120.6(4) . .
C7 C6 H6 119.7 . .
C5 C6 H6 119.7 . .
C2 C7 C6 120.9(4) . .
C2 C7 H7 119.6 . .
C6 C7 H7 119.6 . .
N1 C8 C9 123.8(3) . .
N1 C8 C5 115.9(3) . .
C9 C8 C5 120.2(3) . .
C8 C9 C10 118.6(4) . .
C8 C9 H9 120.7 . .
C10 C9 H9 120.7 . .
C9 C10 C9 117.9(5) 5_565 .
C9 C10 C11 121.1(3) 5_565 .
C9 C10 C11 121.1(3) . .
C12 C11 C12 113.9(8) 5_565 .
C12 C11 C10 123.0(4) 5_565 .
C12 C11 C10 123.0(4) . .
C11 C12 C12 123.0(4) . 21
C11 C12 H12 118.5 . .
C12 C12 H12 118.5 21 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Zr1 O3 2.061(2) 3_655
Zr1 O3 2.061(2) .
Zr1 O1 2.1920(19) 22_565
Zr1 O1 2.1920(19) 21_655
Zr1 O1 2.1920(19) 3_655
Zr1 O1 2.1920(19) .
Zr1 O4 2.306(3) .
Zr1 O4 2.306(3) 3_655
Zr1 Zr2 3.4890(3) 26_565
Zr1 Zr2 3.4890(3) 20_656
Zr1 Zr2 3.4890(3) .
Zr1 Zr2 3.4890(3) 3_655
Zr2 O3 2.0637(12) .
Zr2 O3 2.0637(12) 26_565
Zr2 O5 2.182(3) .
Zr2 O5 2.182(3) 16_554
Zr2 O4 2.2366(14) 20_656
Zr2 O4 2.2366(14) .
Zr2 O2 2.244(2) .
Zr2 O2 2.244(2) 16_554
Zr2 Zr1 3.4890(3) 26_565
Zr2 Zr2 3.5202(5) 20_656
Zr2 Zr2 3.5202(5) 26_565
O1 C1 1.242(4) .
O2 C1 1.275(4) .
O3 Zr2 2.0637(12) 20_656
O4 Zr2 2.2366(14) 26_565
N1 C8 1.327(4) 5_565
N1 C8 1.327(4) .
C1 C2 1.491(4) .
C2 C7 1.357(5) .
C2 C3 1.367(5) .
C3 C4 1.384(4) .
C3 H3 0.9500 .
C4 C5 1.378(5) .
C4 H4 0.9500 .
C5 C6 1.383(5) .
C5 C8 1.493(5) .
C6 C7 1.377(5) .
C6 H6 0.9500 .
C7 H7 0.9500 .
C8 C9 1.367(5) .
C9 C10 1.393(4) .
C9 H9 0.9500 .
C10 C9 1.393(4) 5_565
C10 C11 1.496(8) .
C11 C12 1.217(7) 5_565
C11 C12 1.217(7) .
C12 C12 1.457(11) 21
C12 H12 0.9500 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O3 Zr1 Zr2 O3 -108.80(15) 3_655 .
O1 Zr1 Zr2 O3 36.33(13) 22_565 .
O1 Zr1 Zr2 O3 169.70(13) 21_655 .
O1 Zr1 Zr2 O3 -78.8(3) 3_655 .
O1 Zr1 Zr2 O3 102.38(13) . .
O4 Zr1 Zr2 O3 -176.24(15) . .
O4 Zr1 Zr2 O3 -38.42(12) 3_655 .
Zr2 Zr1 Zr2 O3 -132.22(12) 26_565 .
Zr2 Zr1 Zr2 O3 -22.26(12) 20_656 .
Zr2 Zr1 Zr2 O3 -77.24(12) 3_655 .
O3 Zr1 Zr2 O3 0.09(6) 3_655 26_565
O3 Zr1 Zr2 O3 108.89(16) . 26_565
O1 Zr1 Zr2 O3 145.22(9) 22_565 26_565
O1 Zr1 Zr2 O3 -81.41(8) 21_655 26_565
O1 Zr1 Zr2 O3 30.1(3) 3_655 26_565
O1 Zr1 Zr2 O3 -148.73(8) . 26_565
O4 Zr1 Zr2 O3 -67.35(9) . 26_565
O4 Zr1 Zr2 O3 70.47(7) 3_655 26_565
Zr2 Zr1 Zr2 O3 -23.33(6) 26_565 26_565
Zr2 Zr1 Zr2 O3 86.63(6) 20_656 26_565
Zr2 Zr1 Zr2 O3 31.65(6) 3_655 26_565
O3 Zr1 Zr2 O5 93.32(13) 3_655 .
O3 Zr1 Zr2 O5 -157.88(17) . .
O1 Zr1 Zr2 O5 -121.55(14) 22_565 .
O1 Zr1 Zr2 O5 11.82(14) 21_655 .
O1 Zr1 Zr2 O5 123.3(3) 3_655 .
O1 Zr1 Zr2 O5 -55.50(14) . .
O4 Zr1 Zr2 O5 25.88(15) . .
O4 Zr1 Zr2 O5 163.70(13) 3_655 .
Zr2 Zr1 Zr2 O5 69.90(13) 26_565 .
Zr2 Zr1 Zr2 O5 179.86(13) 20_656 .
Zr2 Zr1 Zr2 O5 124.88(13) 3_655 .
O3 Zr1 Zr2 O5 -151.02(11) 3_655 16_554
O3 Zr1 Zr2 O5 -42.22(16) . 16_554
O1 Zr1 Zr2 O5 -5.89(12) 22_565 16_554
O1 Zr1 Zr2 O5 127.47(12) 21_655 16_554
O1 Zr1 Zr2 O5 -121.0(3) 3_655 16_554
O1 Zr1 Zr2 O5 60.16(12) . 16_554
O4 Zr1 Zr2 O5 141.54(13) . 16_554
O4 Zr1 Zr2 O5 -80.65(11) 3_655 16_554
Zr2 Zr1 Zr2 O5 -174.44(10) 26_565 16_554
Zr2 Zr1 Zr2 O5 -64.48(11) 20_656 16_554
Zr2 Zr1 Zr2 O5 -119.46(10) 3_655 16_554
O3 Zr1 Zr2 O4 -71.69(8) 3_655 20_656
O3 Zr1 Zr2 O4 37.11(13) . 20_656
O1 Zr1 Zr2 O4 73.44(9) 22_565 20_656
O1 Zr1 Zr2 O4 -153.19(9) 21_655 20_656
O1 Zr1 Zr2 O4 -41.7(3) 3_655 20_656
O1 Zr1 Zr2 O4 139.49(9) . 20_656
O4 Zr1 Zr2 O4 -139.13(11) . 20_656
O4 Zr1 Zr2 O4 -1.31(7) 3_655 20_656
Zr2 Zr1 Zr2 O4 -95.11(7) 26_565 20_656
Zr2 Zr1 Zr2 O4 14.85(7) 20_656 20_656
Zr2 Zr1 Zr2 O4 -40.13(7) 3_655 20_656
O3 Zr1 Zr2 O4 67.44(8) 3_655 .
O3 Zr1 Zr2 O4 176.24(15) . .
O1 Zr1 Zr2 O4 -147.43(10) 22_565 .
O1 Zr1 Zr2 O4 -14.06(9) 21_655 .
O1 Zr1 Zr2 O4 97.4(3) 3_655 .
O1 Zr1 Zr2 O4 -81.38(10) . .
O4 Zr1 Zr2 O4 137.82(11) 3_655 .
Zr2 Zr1 Zr2 O4 44.02(7) 26_565 .
Zr2 Zr1 Zr2 O4 153.98(7) 20_656 .
Zr2 Zr1 Zr2 O4 99.00(7) 3_655 .
O3 Zr1 Zr2 O2 153.89(11) 3_655 .
O3 Zr1 Zr2 O2 -97.31(16) . .
O1 Zr1 Zr2 O2 -60.98(12) 22_565 .
O1 Zr1 Zr2 O2 72.39(12) 21_655 .
O1 Zr1 Zr2 O2 -176.1(3) 3_655 .
O1 Zr1 Zr2 O2 5.07(12) . .
O4 Zr1 Zr2 O2 86.45(13) . .
O4 Zr1 Zr2 O2 -135.73(11) 3_655 .
Zr2 Zr1 Zr2 O2 130.47(10) 26_565 .
Zr2 Zr1 Zr2 O2 -119.57(10) 20_656 .
Zr2 Zr1 Zr2 O2 -174.55(10) 3_655 .
O3 Zr1 Zr2 O2 -16.4(3) 3_655 16_554
O3 Zr1 Zr2 O2 92.4(3) . 16_554
O1 Zr1 Zr2 O2 128.8(3) 22_565 16_554
O1 Zr1 Zr2 O2 -97.9(3) 21_655 16_554
O1 Zr1 Zr2 O2 13.6(4) 3_655 16_554
O1 Zr1 Zr2 O2 -165.2(3) . 16_554
O4 Zr1 Zr2 O2 -83.8(3) . 16_554
O4 Zr1 Zr2 O2 54.0(3) 3_655 16_554
Zr2 Zr1 Zr2 O2 -39.8(3) 26_565 16_554
Zr2 Zr1 Zr2 O2 70.2(3) 20_656 16_554
Zr2 Zr1 Zr2 O2 15.2(3) 3_655 16_554
O3 Zr1 Zr2 Zr1 -31.56(3) 3_655 26_565
O3 Zr1 Zr2 Zr1 77.24(12) . 26_565
O1 Zr1 Zr2 Zr1 113.57(6) 22_565 26_565
O1 Zr1 Zr2 Zr1 -113.06(6) 21_655 26_565
O1 Zr1 Zr2 Zr1 -1.6(3) 3_655 26_565
O1 Zr1 Zr2 Zr1 179.62(6) . 26_565
O4 Zr1 Zr2 Zr1 -99.00(7) . 26_565
O4 Zr1 Zr2 Zr1 38.82(3) 3_655 26_565
Zr2 Zr1 Zr2 Zr1 -54.981(3) 26_565 26_565
Zr2 Zr1 Zr2 Zr1 54.981(3) 20_656 26_565
Zr2 Zr1 Zr2 Zr1 0.0 3_655 26_565
O3 Zr1 Zr2 Zr2 -86.54(3) 3_655 20_656
O3 Zr1 Zr2 Zr2 22.26(12) . 20_656
O1 Zr1 Zr2 Zr2 58.59(6) 22_565 20_656
O1 Zr1 Zr2 Zr2 -168.04(6) 21_655 20_656
O1 Zr1 Zr2 Zr2 -56.6(3) 3_655 20_656
O1 Zr1 Zr2 Zr2 124.64(6) . 20_656
O4 Zr1 Zr2 Zr2 -153.98(7) . 20_656
O4 Zr1 Zr2 Zr2 -16.16(3) 3_655 20_656
Zr2 Zr1 Zr2 Zr2 -109.961(5) 26_565 20_656
Zr2 Zr1 Zr2 Zr2 -54.981(3) 3_655 20_656
O3 Zr1 Zr2 Zr2 23.42(3) 3_655 26_565
O3 Zr1 Zr2 Zr2 132.22(12) . 26_565
O1 Zr1 Zr2 Zr2 168.55(6) 22_565 26_565
O1 Zr1 Zr2 Zr2 -58.08(5) 21_655 26_565
O1 Zr1 Zr2 Zr2 53.4(3) 3_655 26_565
O1 Zr1 Zr2 Zr2 -125.40(6) . 26_565
O4 Zr1 Zr2 Zr2 -44.02(7) . 26_565
O4 Zr1 Zr2 Zr2 93.80(3) 3_655 26_565
Zr2 Zr1 Zr2 Zr2 109.961(5) 20_656 26_565
Zr2 Zr1 Zr2 Zr2 54.981(3) 3_655 26_565
O3 Zr1 O1 C1 -66.0(4) 3_655 .
O3 Zr1 O1 C1 24.5(4) . .
O1 Zr1 O1 C1 110.2(3) 22_565 .
O1 Zr1 O1 C1 -124.5(3) 21_655 .
O1 Zr1 O1 C1 173.2(4) 3_655 .
O4 Zr1 O1 C1 -47.7(4) . .
O4 Zr1 O1 C1 75.4(4) 3_655 .
Zr2 Zr1 O1 C1 -56.9(4) 26_565 .
Zr2 Zr1 O1 C1 43.0(4) 20_656 .
Zr2 Zr1 O1 C1 -7.1(3) . .
Zr2 Zr1 O1 C1 -5.5(6) 3_655 .
O3 Zr2 O2 C1 -40.4(5) . .
O3 Zr2 O2 C1 39.4(6) 26_565 .
O5 Zr2 O2 C1 117.0(5) . .
O5 Zr2 O2 C1 -140.7(5) 16_554 .
O4 Zr2 O2 C1 -86.9(5) 20_656 .
O4 Zr2 O2 C1 34.7(5) . .
O2 Zr2 O2 C1 168.0(5) 16_554 .
Zr1 Zr2 O2 C1 -23.8(7) 26_565 .
Zr1 Zr2 O2 C1 -7.7(4) . .
Zr2 Zr2 O2 C1 -58.5(5) 20_656 .
Zr2 Zr2 O2 C1 37.3(5) 26_565 .
O3 Zr1 O3 Zr2 70.91(10) 3_655 .
O1 Zr1 O3 Zr2 -146.23(12) 22_565 .
O1 Zr1 O3 Zr2 -16.1(2) 21_655 .
O1 Zr1 O3 Zr2 157.88(9) 3_655 .
O1 Zr1 O3 Zr2 -71.96(11) . .
O4 Zr1 O3 Zr2 2.50(10) . .
O4 Zr1 O3 Zr2 139.32(13) 3_655 .
Zr2 Zr1 O3 Zr2 40.43(10) 26_565 .
Zr2 Zr1 O3 Zr2 141.8(2) 20_656 .
Zr2 Zr1 O3 Zr2 101.38(10) 3_655 .
O3 Zr1 O3 Zr2 -70.91(10) 3_655 20_656
O1 Zr1 O3 Zr2 71.96(11) 22_565 20_656
O1 Zr1 O3 Zr2 -157.88(9) 21_655 20_656
O1 Zr1 O3 Zr2 16.1(2) 3_655 20_656
O1 Zr1 O3 Zr2 146.23(12) . 20_656
O4 Zr1 O3 Zr2 -139.32(13) . 20_656
O4 Zr1 O3 Zr2 -2.50(10) 3_655 20_656
Zr2 Zr1 O3 Zr2 -101.38(10) 26_565 20_656
Zr2 Zr1 O3 Zr2 -141.8(2) . 20_656
Zr2 Zr1 O3 Zr2 -40.43(10) 3_655 20_656
O3 Zr2 O3 Zr1 -69.94(11) 26_565 .
O5 Zr2 O3 Zr1 35.3(3) . .
O5 Zr2 O3 Zr1 144.86(12) 16_554 .
O4 Zr2 O3 Zr1 -140.11(14) 20_656 .
O4 Zr2 O3 Zr1 -2.56(10) . .
O2 Zr2 O3 Zr1 73.99(13) . .
O2 Zr2 O3 Zr1 -144.86(16) 16_554 .
Zr1 Zr2 O3 Zr1 -100.30(10) 26_565 .
Zr2 Zr2 O3 Zr1 -141.2(2) 20_656 .
Zr2 Zr2 O3 Zr1 -40.08(10) 26_565 .
O3 Zr2 O3 Zr2 71.27(10) 26_565 20_656
O5 Zr2 O3 Zr2 176.6(2) . 20_656
O5 Zr2 O3 Zr2 -73.92(13) 16_554 20_656
O4 Zr2 O3 Zr2 1.11(12) 20_656 20_656
O4 Zr2 O3 Zr2 138.65(13) . 20_656
O2 Zr2 O3 Zr2 -144.80(15) . 20_656
O2 Zr2 O3 Zr2 -3.6(3) 16_554 20_656
Zr1 Zr2 O3 Zr2 40.91(11) 26_565 20_656
Zr1 Zr2 O3 Zr2 141.2(2) . 20_656
Zr2 Zr2 O3 Zr2 101.13(11) 26_565 20_656
O3 Zr2 O4 Zr2 -101.39(11) . 26_565
O3 Zr2 O4 Zr2 -0.94(10) 26_565 26_565
O5 Zr2 O4 Zr2 100.27(14) . 26_565
O5 Zr2 O4 Zr2 -176.1(2) 16_554 26_565
O4 Zr2 O4 Zr2 -51.81(7) 20_656 26_565
O2 Zr2 O4 Zr2 176.11(14) . 26_565
O2 Zr2 O4 Zr2 48.34(16) 16_554 26_565
Zr1 Zr2 O4 Zr2 -21.02(10) 26_565 26_565
Zr1 Zr2 O4 Zr2 -103.49(12) . 26_565
Zr2 Zr2 O4 Zr2 -81.05(9) 20_656 26_565
O3 Zr2 O4 Zr1 2.10(8) . .
O3 Zr2 O4 Zr1 102.55(10) 26_565 .
O5 Zr2 O4 Zr1 -156.24(12) . .
O5 Zr2 O4 Zr1 -72.6(3) 16_554 .
O4 Zr2 O4 Zr1 51.67(6) 20_656 .
O2 Zr2 O4 Zr1 -80.40(11) . .
O2 Zr2 O4 Zr1 151.82(9) 16_554 .
Zr1 Zr2 O4 Zr1 82.47(6) 26_565 .
Zr2 Zr2 O4 Zr1 22.43(6) 20_656 .
Zr2 Zr2 O4 Zr1 103.49(12) 26_565 .
O3 Zr1 O4 Zr2 -104.14(9) 3_655 .
O3 Zr1 O4 Zr2 -2.12(8) . .
O1 Zr1 O4 Zr2 52.54(15) 22_565 .
O1 Zr1 O4 Zr2 166.36(9) 21_655 .
O1 Zr1 O4 Zr2 -158.80(8) 3_655 .
O1 Zr1 O4 Zr2 87.38(7) . .
O4 Zr1 O4 Zr2 -53.13(6) 3_655 .
Zr2 Zr1 O4 Zr2 -106.26(12) 26_565 .
Zr2 Zr1 O4 Zr2 -22.62(6) 20_656 .
Zr2 Zr1 O4 Zr2 -83.64(6) 3_655 .
O3 Zr1 O4 Zr2 2.12(8) 3_655 26_565
O3 Zr1 O4 Zr2 104.14(9) . 26_565
O1 Zr1 O4 Zr2 158.80(8) 22_565 26_565
O1 Zr1 O4 Zr2 -87.38(7) 21_655 26_565
O1 Zr1 O4 Zr2 -52.54(15) 3_655 26_565
O1 Zr1 O4 Zr2 -166.36(9) . 26_565
O4 Zr1 O4 Zr2 53.13(6) 3_655 26_565
Zr2 Zr1 O4 Zr2 83.64(6) 20_656 26_565
Zr2 Zr1 O4 Zr2 106.26(12) . 26_565
Zr2 Zr1 O4 Zr2 22.62(6) 3_655 26_565
Zr1 O1 C1 O2 4.6(7) . .
Zr1 O1 C1 C2 -175.3(3) . .
Zr2 O2 C1 O1 5.8(8) . .
Zr2 O2 C1 C2 -174.3(3) . .
O1 C1 C2 C7 165.5(5) . .
O2 C1 C2 C7 -14.4(7) . .
O1 C1 C2 C3 -10.9(7) . .
O2 C1 C2 C3 169.2(4) . .
C7 C2 C3 C4 4.9(8) . .
C1 C2 C3 C4 -178.7(4) . .
C2 C3 C4 C5 -6.0(8) . .
C3 C4 C5 C6 3.7(8) . .
C3 C4 C5 C8 -176.9(5) . .
C4 C5 C6 C7 -0.5(9) . .
C8 C5 C6 C7 -179.9(5) . .
C3 C2 C7 C6 -1.7(8) . .
C1 C2 C7 C6 -178.1(5) . .
C5 C6 C7 C2 -0.5(9) . .
C8 N1 C8 C9 -0.8(5) 5_565 .
C8 N1 C8 C5 176.2(6) 5_565 .
C4 C5 C8 N1 -29.6(8) . .
C6 C5 C8 N1 149.8(5) . .
C4 C5 C8 C9 147.6(6) . .
C6 C5 C8 C9 -33.0(9) . .
N1 C8 C9 C10 1.5(10) . .
C5 C8 C9 C10 -175.4(5) . .
C8 C9 C10 C9 -0.7(5) . 5_565
C8 C9 C10 C11 179.3(5) . .
C9 C10 C11 C12 9.3(6) 5_565 5_565
C9 C10 C11 C12 -170.7(6) . 5_565
C9 C10 C11 C12 -170.7(6) 5_565 .
C9 C10 C11 C12 9.3(6) . .
C12 C11 C12 C12 0.000(3) 5_565 21
C10 C11 C12 C12 180.000(3) . 21
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 -0.026 0.145 -0.004 22558 4954 ' '
